Properties of Non-Structural Concrete Made with Mixed Recycled Aggregates and Low Cement Content Antonio López-Uceda 1 , Jesús Ayuso 1, *, Martin López 1 , José Ramón Jimenez 1 , Francisco Agrela 1 and María José Sierra 2 1
Construction Engineering, University of Córdoba, Ed. Leonardo Da Vinci, Campus of Rabanales, Córdoba 14071, Spain; [email protected]
(A.L.-U.); [email protected]
(M.L.); [email protected]
(J.R.J.); [email protected]
(F.A.) Public Works Agency and Regional Ministry of Public Works and Housing of the Regional Government of Andalusia, Sevilla 41013, Spain; [email protected]
Correspondence: [email protected]
; Tel.: +34-957-218-452; Fax: +34-957-218-550
Academic Editor: Jorge de Brito Received: 21 September 2015; Accepted: 15 January 2016; Published: 26 January 2016
Abstract: In spite of not being legally accepted in most countries, mixed recycled aggregates (MRA) could be a suitable raw material for concrete manufacturing. The aims of this research were as follows: (i) to analyze the effect of the replacement ratio of natural coarse aggregates with MRA, the amount of ceramic particles in MRA, and the amount of cement, on the mechanical and physical properties of a non-structural concrete made with a low cement content; and (ii) to verify if it is possible to achieve a low-strength concrete that replaces a greater amount of natural aggregate with MRA and that has a low cement content. Two series of concrete mixes were manufactured using 180 and 200 kg/m3 of CEM II/A-V 42.5 R type Portland cement. Each series included seven concrete mixes: one with natural aggregates; two MRA with different ceramic particle contents; and one for each coarse aggregate replacement ratio (20%, 40%, and 100%). To study their properties, compressive and splitting tensile strength, modulus of elasticity, density, porosity, water penetration, and sorptivity, tests were performed. The results confirmed that the main factors affecting the properties analyzed in this research are the amount of cement and the replacement ratio; the two MRAs used in this work presented a similar influence on the properties. A non-structural, low-strength concrete (15 MPa) with an MRA replacement ratio of up to 100% for 200 kg/m3 of cement was obtained. This type of concrete could be applied in the construction of ditches, sidewalks, and other similar civil works. Keywords: mixed recycled aggregate; ceramics; low cement content; non-structural concrete; mechanical properties; physical properties
1. Introduction Most of the CO2 -equivalent produced to manufacture concrete comes from cement production; over 400 kg of CO2 -equivalent is generated per m3 of concrete [1,2], and is also responsible for 5% of all anthropogenic CO2 emissions . In the European Union, 900 million tonnes of cement were produced in 2008 . In the same year, CO2 equivalent emissions reached 101 million tonnes in the cement production sector . This results in a high contribution to the emission of greenhouse gases, and contributes greatly to global warming. Construction and demolition waste (CDW) represents almost a third of the total waste generated in the EU . If CDW is not properly managed and is instead deposited in landfills, it can cause serious environmental problems, such as the release of contaminants that pollute surface and ground water [6,7]. Moreover, the recycling and reuse of CDW in new building materials require less energy consumption, reduce CO2 equivalent emissions, and, as a result, benefit the environment. Materials 2016, 9, 74; doi:10.3390/ma9020074
Materials 2016, 9, 74
2 of 19
Knoeri et al.  significantly reduced the environmental impact of recycled lean concrete by using 100% mixed rubble aggregates instead of conventional lean concrete. To promote the recycling and reuse of CDW, the Waste Framework Directive 2008/98/EC has mandated a 70% minimum CDW reuse and recycling rate by 2020. In Spain, the Second National Plan for CDW 2008–2015  was developed to promote the recycling of this waste. This plan set a goal of achieving a recycling rate of 35% in 2015. CDW consists of ceramic particles, mortar, concrete, and natural aggregates, as well as minor amounts of asphaltic material, gypsum, and impurities such as wood, metal particles, paper, and plastics. There are two major classifications of CDW aggregates, depending on their origin: recycled concrete aggregate (RCA), produced by crushing concrete, and mixed recycled aggregate (MRA), including at least 5% ceramic particles by weight. In Spain, RCA represents approximately 15%–20% and MRA approximately 80% of the total CDW aggregates produced . In Spain, Structural Concrete Code EHE-08  is the regulatory framework that sets the requirements for all materials used in concrete manufacturing, including recycled aggregates (RA). Among them, the fine fraction of RA is not allowed to be used in concrete manufacturing. The code only permits the use of the coarse fraction of RCA, which limits the replacement ratio of structural concrete to 20%. For non-structural concrete, coarse natural aggregates can be replaced by RCA up to 100%. Both cases exclude concretes manufactured using MRA. The standards in other countries, such as Germany, the United Kingdom, and Portugal, permit the partial or total use of MRA as the coarse fraction in non-structural concrete manufacturing, with different requirements in each country . EHE-08 limits the minimum characteristic strength of non-structural concrete to 15 MPa and minimum cement content to 150 kg/m3 . Because non-structural concretes are not steel reinforced, the EHE-08 code does not include any reference to the environment. 2. Literary Review The possibility of using the coarse fraction of RCA for the partial or total replacement of the coarse fraction of natural aggregates (NA) in the manufacture of structural concrete has been studied by many researchers. It has been observed [13,14] that replacement ratios up to approximately 20% of RCA have marginal effects on the development of strength in concrete. Exteberría et al.  found that the strength of concrete made entirely with RCA was 20%–25% lower than conventional concrete after 28 days. Thomas et al.  found that a 20% replacement ratio led to minimal differences in water penetration under pressure and density values, approximately 5% lower than those of the control concrete. Malešev et al.  found a 44% increase in water absorption by sorptivity with total replacement using RCA with respect to the control concrete. The effect of recycled aggregates made of pure ceramics has been explored by several authors, who used crushed bricks to replace the coarse fraction of NA. Their results are somewhat diverse. Brito et al.  measured strength losses of 45% with a replacement ratio of 100%, while Cachim  found up to 20% strength losses with 30% replacement. Similar results were found by Yang et al. , who observed a 10% reduction in strength with 20% replacement compared to the control concrete. Guerra et al.  obtained similar values when replacing up to 9% of the NA with recycled ceramic materials from sanitary porcelain debris. However, a few studies have also been dedicated to the possibility of using MRA as a total or partial replacement material for the coarse fraction in the manufacture of concrete [21–27]. The objective of these studies was to obtain a structural concrete with a compressive strength greater than 25 MPa. The amount of cement used ranged from 240 kg/m3 to more than 300 kg/m3 , so the amount of cement under 240 kg/m3 remains unexplored in studies with MRA incorporation in concrete. It was found that concrete made with MRA has a higher porosity, water absorption, and permeability and a lower strength than the control concretes that were made with NA and the same concrete mix composition.
Materials 2016, 9, 74
3 of 19
The objectives of this work were as follows: (i) to analyze the mechanical and physical properties of a non-structural concrete made with MRA and a low cement content, and to study the effect of Materials 2016, 9, 74 3 of 18 three factors: the replacement ratio of natural coarse aggregate by coarse MRA at four levels (0%, 20%, (0%, 20%, 40%, and 100%), the amount of ceramic particles in the MRA at two levels (14% and 30%) 40%, and 100%), the amount of ceramic particles in the MRA at two levels (14% and 30%) and the and the of amount at two (180 and 3200 kg/m3 of concrete); (ii) verify if it to is amount cementof atcement two levels (180levels and 200 kg/m of concrete); and (ii) to and verify if to it is possible possible to achieve a low strength concrete that replaces a greater amount of natural aggregate with achieve a low strength concrete that replaces a greater amount of natural aggregate with MRA that has aMRA that has a low cement content. This non‐structural concrete could be applied to build ditches, low cement content. This non-structural concrete could be applied to build ditches, floors, sidewalks, floors, sidewalks, and which paving blocks, for which a high mechanical is of not necessary. and paving blocks, for a high mechanical strength is not necessary. strength The results this research The results of this research might have the double environmental benefit of reducing CO 2 emissions might have the double environmental benefit of reducing CO2 emissions by reducing the amount of by reducing the amount an of RA cement and by recycling an RA of the low quality, which represents the cement and by recycling of low quality, which represents highest percentage of the CDW highest percentage of the CDW aggregates produced. aggregates produced. 3. Materials and Experimental Details 3. Materials and Experimental Details 3.1. Materials 3.1. Materials 3.1.1. Mixed Recycled Aggregates 3.1.1. Mixed Recycled Aggregates Two recycled aggregates (MRA1 and MRA2) with different percentages of ceramic Two mixed mixed recycled aggregates (MRA1 and MRA2) with different percentages of particles ceramic collected on different days from a CDW treatment plant located in Córdoba (South of Spain) were particles collected on different days from a CDW treatment plant located in Córdoba (South of Spain) used. These aggregates were by-products of the demolition of residential buildings. The grain size were used. These aggregates were by‐products of the demolition of residential buildings. The grain distribution of the materials is shown in Figure 1. Both materials were obtained by sieving the 0–25 mm size distribution of the materials is shown in Figure 1. Both materials were obtained by sieving the fraction produced in the treatment plant. 0–25 mm fraction produced in the treatment plant.
Figure 1. Particle size distribution of aggregates. Mixed recycled aggregates (MRA1 and MRA2). Figure 1. Particle size distribution of aggregates. Mixed recycled aggregates (MRA1 and MRA2).
Table 1 shows the physical and chemical properties as well as the main constituents of the recycled Table 1 shows the physical and chemical properties as well as the main constituents of the recycled coarse aggregate with the RA constraints of the Spanish Code EHE‐08. Only the water absorption coarse aggregate with the RA constraints of the Spanish Code EHE-08. Only the water absorption requirement was not satisfied by MRA2, although, for RILEM (The International Union of Laboratories requirement was not satisfied by MRA2, although, for RILEM (The International Union of Laboratories and Experts in Construction Materials, Systems and Structures) , the limit is less restrictive and and Experts in Construction Materials, Systems and Structures) , the limit is less restrictive and up up to 20% is allowed. It was noted that the amount of ceramic particles in MRA2 was greater than to 20% allowed. was noted that the amount of ceramic particles in MRA2 was greater thanEHE‐08 that in that in isMRA1, so Itthat, the absorption was higher in MRA2. MRA2 complies with the MRA1, so that, the absorption was higher in MRA2. MRA2 complies with the EHE-08 requirements, requirements, whereas MRA1 does not, as its total sulfur content slightly exceeds the EHE‐08 limit. whereas MRA1 does not, as its total sulfur content slightly exceeds the EHE-08 limit. In the literature In the literature review, different classifications have been proposed based on properties or compositions review, different classifications have been proposed based on properties or compositions of the two of the two MRA. Agrela et al.  established a classification for RA that depends on the ceramic and MRA. Agrela et al.  established a classification for RA that depends on the ceramic and concrete concrete particle content. In this scheme, MRA1 was classified as mixed recycled aggregate (MixRA), particle In this scheme, MRA1 was10%–30% classified by as mixed recycled (MixRA), because content. its ceramic content was between weight. MRA2 aggregate was classified as a because ceramic its ceramic content was between 10%–30% by weight. MRA2 was classified as a ceramic recycled recycled aggregate (CerRA) because its ceramic content was over 30% by weight. Silva et al.  aggregate because its ceramic content over 30% by weight. Silva et al.absorption,  suggested suggested (CerRA) a different RA classification based was on the oven‐dried density, water and aLos different RA(LA) classification based on the oven-dried density, water and Los Angeles Angeles abrasion value. In the latter scheme, MRA1 was absorption, classified as B‐II because its −3 oven‐dried density was higher than 2.2 Mg∙m , and its water absorption and LA values were lower than 6.5% and 45, respectively. Conversely, MRA2 was classified as C‐I because its oven‐dried density was over 2.0 Mg∙m−3, and its water absorption and LA values were lower than 10.5% and 50, respectively.
Materials 2016, 9, 74
4 of 19
(LA) abrasion value. In the latter scheme, MRA1 was classified as B-II because its oven-dried density was higher than 2.2 Mg¨ m´3 , and its water absorption and LA values were lower than 6.5% and 45, respectively. Conversely, MRA2 was classified as C-I because its oven-dried density was over 2.0 Mg¨ m´3 , and its water absorption and LA values were lower than 10.5% and 50, respectively. Table 1. Physical, chemical properties and components of mixed recycled aggregates (MRA). SSD: Saturated surface dry. Physical Properties
According to Standard
Water absorption (%) Oven-dried density (Mg/m3 ) SSD density (Mg/m3 ) Flakiness index (%) Los Angeles Abrasion test Freeze-thaw resistance (%)
UNE-EN 1097-6:2014  UNE-EN 1097-6:2014  UNE-EN 1097-6:2014  UNE-EN 933-3:2012  UNE-EN 1097-2:2010  UNE-EN 1367-2:2010 
6.1 2.24 2.38 10.8 35.6 5.2
9.0 2.08 2.27 14.7 32.3 14.0